#------------------------------------------------------------------------------
#$Date: 2023-03-26 11:09:57 +0300 (Sun, 26 Mar 2023) $
#$Revision: 282068 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/29/2102958.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2102958
loop_
_publ_author_name
'Boysen, H.'
'Lerch, M.'
'Stys, A.'
'Senyshyn, A.'
_publ_contact_author_address
;Department für Geo- und Umweltwissenschaften,
Sektion Kristallographie, LMU München,
 Am Coulombwall 1, 85748 Garching, Germany
;
_publ_contact_author_email       boysen@lmu.de
_publ_contact_author_fax         498928914015
_publ_contact_author_name        'Hans Boysen'
_publ_contact_author_phone       498928914040
_publ_section_title
;
 Structure and oxygen mobility in mayenite (Ca₁₂Al₁₄O₃₃): a
 high-temperature neutron powder diffraction study
;
_journal_coeditor_code           WS5057
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              675
_journal_page_last               682
_journal_paper_doi               10.1107/S0108768107030005
_journal_volume                  63
_journal_year                    2007
_chemical_compound_source        Synthetic
_chemical_formula_moiety         'Al14  Ca12  O33'
_chemical_formula_sum            'Al14 Ca12 O33'
_chemical_formula_weight         1386.7
_chemical_name_mineral           mayenite
_space_group_IT_number           220
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   12.0585
_cell_length_b                   12.0585
_cell_length_c                   12.0585
_cell_measurement_temperature    1323
_cell_volume                     1753.395
_computing_publication_material  '(Jana2000; Petricek and Dusek, 2000)'
_computing_structure_refinement  '(Jana2000; Petricek and Dusek, 2000)'
_database_code_amcsd             0009967
_diffrn_ambient_temperature      1323
_diffrn_measurement_device_type  'Debye Scherrer'
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.548
_exptl_absorpt_coefficient_mu    0.001
_exptl_absorpt_process_details
'(Jana2000; Petricek, Dusek & Palatinus, 2000)'
_exptl_crystal_density_diffrn    2.6256
_exptl_crystal_F_000             1370
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.43
_refine_ls_number_parameters     41
_refine_ls_R_factor_all          0.0404
_refine_ls_R_factor_gt           0.0309
_refine_ls_shift/su_max          0.0171
_refine_ls_shift/su_mean         0.0047
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0210
_refine_ls_wR_factor_ref         0.0219
_cod_data_source_file            ws5057.cif
_cod_data_source_block           IV
_cod_depositor_comments
;
 Renaming the _chemical_name_common data item to _chemical_name_mineral
 and removing the '?' prefix from the data value.

 Antanas Vaitkus,
 2018-08-28
;
_cod_original_cell_volume        1753.396
_cod_original_sg_symbol_Hall     'I -4bd;2ab;3'
_cod_database_code               2102958
loop_
_symmetry_equiv_pos_site_id
_space_group_symop_operation_xyz
1 x,y,z
2 1/4+y,3/4-x,1/4-z
3 x,-y,1/2-z
4 z,x,y
5 -x,1/2-y,z
6 1/4-y,3/4-x,3/4+z
7 1/4+x,3/4-z,1/4-y
8 1/4-y,1/4+x,3/4-z
9 -x,1/2+y,1/2-z
10 -z,1/2-x,y
11 1/4+y,1/4+x,1/4+z
12 1/4-x,1/4+z,3/4-y
13 z,-x,1/2-y
14 1/4-x,3/4-z,3/4+y
15 -z,1/2+x,1/2-y
16 1/4+x,1/4+z,1/4+y
17 1/4-z,1/4+y,3/4-x
18 y,z,x
19 1/4+z,3/4-y,1/4-x
20 -y,1/2-z,x
21 1/4-z,3/4-y,3/4+x
22 -y,1/2+z,1/2-x
23 1/4+z,1/4+y,1/4+x
24 y,-z,1/2-x
25 1/2+x,1/2+y,1/2+z
26 3/4+y,1/4-x,3/4-z
27 1/2+x,1/2-y,-z
28 1/2+z,1/2+x,1/2+y
29 1/2-x,-y,1/2+z
30 3/4-y,1/4-x,1/4+z
31 3/4+x,1/4-z,3/4-y
32 3/4-y,3/4+x,1/4-z
33 1/2-x,y,-z
34 1/2-z,-x,1/2+y
35 3/4+y,3/4+x,3/4+z
36 3/4-x,3/4+z,1/4-y
37 1/2+z,1/2-x,-y
38 3/4-x,1/4-z,1/4+y
39 1/2-z,x,-y
40 3/4+x,3/4+z,3/4+y
41 3/4-z,3/4+y,1/4-x
42 1/2+y,1/2+z,1/2+x
43 3/4+z,1/4-y,3/4-x
44 1/2-y,-z,1/2+x
45 3/4-z,1/4-y,1/4+x
46 1/2-y,z,-x
47 3/4+z,3/4+y,3/4+x
48 1/2+y,1/2-z,-x
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
Ca Ca 0.1456(6) 0 0.25 0.047(2) Uani d 0.926(13)
Al Al1 0.0183(3) 0.0183(3) 0.0183(3) 0.0253(9) Uani d 1
Al Al2 0.875 0 0.25 0.0199(14) Uani d 1
O O1 0.78779(18) 0.10087(16) 0.30547(16) 0.0430(9) Uani d 1
O O2 -0.06399(16) -0.06399(16) -0.06399(16) 0.0428(6) Uani d 1
O O3 0.375 0 0.25 0.28(7) Uiso d 0.15(3)
Ca Cas 0.212(7) 0 0.25 0.05(2) Uiso d 0.074(13)
loop_
_atom_type_symbol
_atom_type_scat_source
Ca International_Tables_Vol_C
Al International_Tables_Vol_C
O International_Tables_Vol_C
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O1 Ca O1 6_554 8_545 178.0(3) yes
O1 Ca O1 6_554 36_545 66.83(12) yes
O1 Ca O1 6_554 38_555 115.0(2) yes
O1 Ca O2 6_554 2_545 97.62(8) yes
O1 Ca O2 6_554 11_555 81.97(8) yes
O1 Ca O3 6_554 . 88.99(17) yes
O1 Ca Cas 6_554 . 88.99(17) yes
O1 Ca O1 8_545 6_554 178.0(3) yes
O1 Ca O1 8_545 36_545 115.0(2) yes
O1 Ca O1 8_545 38_555 66.83(12) yes
O1 Ca O2 8_545 2_545 81.97(8) yes
O1 Ca O2 8_545 11_555 97.62(8) yes
O1 Ca O3 8_545 . 88.99(17) yes
O1 Ca Cas 8_545 . 88.99(17) yes
O1 Ca O1 36_545 6_554 66.83(12) yes
O1 Ca O1 36_545 8_545 115.0(2) yes
O1 Ca O1 36_545 38_555 64.22(18) yes
O1 Ca O2 36_545 2_545 123.8(2) yes
O1 Ca O2 36_545 11_555 77.56(11) yes
O1 Ca O3 36_545 . 147.89(9) yes
O1 Ca Cas 36_545 . 147.89(9) yes
O1 Ca O1 38_555 6_554 115.0(2) yes
O1 Ca O1 38_555 8_545 66.83(12) yes
O1 Ca O1 38_555 36_545 64.22(18) yes
O1 Ca O2 38_555 2_545 77.56(11) yes
O1 Ca O2 38_555 11_555 123.8(2) yes
O1 Ca O3 38_555 . 147.89(9) yes
O1 Ca Cas 38_555 . 147.89(9) yes
O2 Ca O2 2_545 11_555 156.8(3) yes
O2 Ca O3 2_545 . 78.40(17) yes
O2 Ca Cas 2_545 . 78.40(17) yes
O2 Ca O2 11_555 2_545 156.8(3) yes
O2 Ca O3 11_555 . 78.40(17) yes
O2 Ca Cas 11_555 . 78.40(17) yes
O3 Ca Cas . . 0 yes
O1 Al1 O1 6_554 36_545 102.15(18) yes
O1 Al1 O1 6_554 43_455 102.15(18) yes
O1 Al1 O2 6_554 . 116.06(19) yes
O1 Al1 O1 36_545 6_554 102.15(18) yes
O1 Al1 O1 36_545 43_455 102.15(18) yes
O1 Al1 O2 36_545 . 116.06(19) yes
O1 Al1 O1 43_455 6_554 102.15(18) yes
O1 Al1 O1 43_455 36_545 102.15(18) yes
O1 Al1 O2 43_455 . 116.06(19) yes
O1 Al2 O1 . 3_555 105.71(10) yes
O1 Al2 O1 . 36_645 111.39(9) yes
O1 Al2 O1 . 38_655 111.39(9) yes
O1 Al2 O1 3_555 . 105.71(10) yes
O1 Al2 O1 3_555 36_645 111.39(9) yes
O1 Al2 O1 3_555 38_655 111.39(9) yes
O1 Al2 O1 36_645 . 111.39(9) yes
O1 Al2 O1 36_645 3_555 111.39(9) yes
O1 Al2 O1 36_645 38_655 105.71(10) yes
O1 Al2 O1 38_655 . 111.39(9) yes
O1 Al2 O1 38_655 3_555 111.39(9) yes
O1 Al2 O1 38_655 36_645 105.71(10) yes
Ca O1 Ca 26_555 36_545 95.63(11) yes
Ca O1 Al1 26_555 30_555 99.2(2) yes
Ca O1 Al2 26_555 . 120.29(17) yes
Ca O1 O1 26_555 3_555 119.23(19) yes
Ca O1 O1 26_555 36_645 141.80(11) yes
Ca O1 O1 26_555 38_655 87.95(13) yes
Ca O1 O1 26_555 15_645 60.42(17) yes
Ca O1 O1 26_555 48_556 103.71(11) yes
Ca O1 O2 26_555 30_555 118.83(19) yes
Ca O1 Cas 26_555 26_555 19(2) yes
Ca O1 Ca 36_545 26_555 95.63(11) yes
Ca O1 Al1 36_545 30_555 91.53(14) yes
Ca O1 Al2 36_545 . 95.04(12) yes
Ca O1 O1 36_545 3_555 57.89(10) yes
Ca O1 O1 36_545 36_645 111.27(10) yes
Ca O1 O1 36_545 38_655 111.27(11) yes
Ca O1 O1 36_545 15_645 98.05(11) yes
Ca O1 O1 36_545 48_556 52.74(8) yes
Ca O1 O2 36_545 30_555 111.70(9) yes
Ca O1 Cas 36_545 26_555 86.8(9) yes
Al1 O1 Al2 30_555 . 138.96(15) yes
Al1 O1 O1 30_555 3_555 131.11(14) yes
Al1 O1 O1 30_555 36_645 106.39(13) yes
Al1 O1 O1 30_555 38_655 155.43(15) yes
Al1 O1 O1 30_555 15_645 38.92(11) yes
Al1 O1 O1 30_555 48_556 38.92(11) yes
Al1 O1 O2 30_555 30_555 31.40(11) yes
Al1 O1 Cas 30_555 26_555 115.9(17) yes
Al2 O1 O1 . 3_555 37.15(6) yes
Al2 O1 O1 . 36_645 34.31(6) yes
Al2 O1 O1 . 38_655 34.31(6) yes
Al2 O1 O1 . 15_645 166.76(12) yes
Al2 O1 O1 . 48_556 128.49(10) yes
Al2 O1 O2 . 30_555 110.77(10) yes
Al2 O1 Cas . 26_555 104.9(16) yes
O1 O1 O1 3_555 36_645 61.15(7) yes
O1 O1 O1 3_555 38_655 61.15(7) yes
O1 O1 O1 3_555 15_645 155.87(11) yes
O1 O1 O1 3_555 48_556 99.33(9) yes
O1 O1 O2 3_555 30_555 121.72(9) yes
O1 O1 Cas 3_555 26_555 100.6(19) yes
O1 O1 O1 36_645 3_555 61.15(7) yes
O1 O1 O1 36_645 38_655 57.69(7) yes
O1 O1 O1 36_645 15_645 136.16(9) yes
O1 O1 O1 36_645 48_556 114.07(9) yes
O1 O1 O2 36_645 30_555 76.62(7) yes
O1 O1 Cas 36_645 26_555 133.4(11) yes
O1 O1 O1 38_655 3_555 61.15(7) yes
O1 O1 O1 38_655 36_645 57.69(7) yes
O1 O1 O1 38_655 15_645 139.02(9) yes
O1 O1 O1 38_655 48_556 160.47(10) yes
O1 O1 O2 38_655 30_555 125.66(9) yes
O1 O1 Cas 38_655 26_555 75.9(12) yes
O1 O1 O1 15_645 3_555 155.87(11) yes
O1 O1 O1 15_645 36_645 136.16(9) yes
O1 O1 O1 15_645 38_655 139.02(9) yes
O1 O1 O1 15_645 48_556 60.00(7) yes
O1 O1 O2 15_645 30_555 62.23(7) yes
O1 O1 Cas 15_645 26_555 78.0(18) yes
O1 O1 O1 48_556 3_555 99.33(9) yes
O1 O1 O1 48_556 36_645 114.07(9) yes
O1 O1 O1 48_556 38_655 160.47(10) yes
O1 O1 O1 48_556 15_645 60.00(7) yes
O1 O1 O2 48_556 30_555 62.23(7) yes
O1 O1 Cas 48_556 26_555 110.9(7) yes
O2 O1 Cas 30_555 26_555 137.5(19) yes
Ca O2 Ca 31_454 32_445 99.96(18) yes
Ca O2 Ca 31_454 21_544 99.96(18) yes
Ca O2 Al1 31_454 . 117.83(16) yes
Ca O2 O1 31_454 6_554 126.21(17) yes
Ca O2 O1 31_454 36_545 132.06(8) yes
Ca O2 O1 31_454 43_455 85.42(11) yes
Ca O2 Cas 31_454 31_454 19(2) yes
Ca O2 Cas 31_454 32_445 93.9(7) yes
Ca O2 Cas 31_454 21_544 119(2) yes
Ca O2 Ca 32_445 31_454 99.96(18) yes
Ca O2 Ca 32_445 21_544 99.96(18) yes
Ca O2 Al1 32_445 . 117.83(16) yes
Ca O2 O1 32_445 6_554 132.06(8) yes
Ca O2 O1 32_445 36_545 85.42(11) yes
Ca O2 O1 32_445 43_455 126.21(17) yes
Ca O2 Cas 32_445 31_454 119(2) yes
Ca O2 Cas 32_445 32_445 19(2) yes
Ca O2 Cas 32_445 21_544 93.9(7) yes
Ca O2 Ca 21_544 31_454 99.96(18) yes
Ca O2 Ca 21_544 32_445 99.96(18) yes
Ca O2 Al1 21_544 . 117.83(16) yes
Ca O2 O1 21_544 6_554 85.42(11) yes
Ca O2 O1 21_544 36_545 126.21(17) yes
Ca O2 O1 21_544 43_455 132.06(8) yes
Ca O2 Cas 21_544 31_454 93.9(7) yes
Ca O2 Cas 21_544 32_445 119(2) yes
Ca O2 Cas 21_544 21_544 19(2) yes
Al1 O2 O1 . 6_554 32.54(12) yes
Al1 O2 O1 . 36_545 32.54(12) yes
Al1 O2 O1 . 43_455 32.54(12) yes
Al1 O2 Cas . 31_454 106.2(14) yes
Al1 O2 Cas . 32_445 106.2(14) yes
Al1 O2 Cas . 21_544 106.2(14) yes
O1 O2 O1 6_554 36_545 55.53(7) yes
O1 O2 O1 6_554 43_455 55.53(7) yes
O1 O2 Cas 6_554 31_454 108(2) yes
O1 O2 Cas 6_554 32_445 129.9(5) yes
O1 O2 Cas 6_554 21_544 75.9(10) yes
O1 O2 O1 36_545 6_554 55.53(7) yes
O1 O2 O1 36_545 43_455 55.53(7) yes
O1 O2 Cas 36_545 31_454 129.9(5) yes
O1 O2 Cas 36_545 32_445 75.9(10) yes
O1 O2 Cas 36_545 21_544 108(2) yes
O1 O2 O1 43_455 6_554 55.53(7) yes
O1 O2 O1 43_455 36_545 55.53(7) yes
O1 O2 Cas 43_455 31_454 75.9(10) yes
O1 O2 Cas 43_455 32_445 108(2) yes
O1 O2 Cas 43_455 21_544 129.9(5) yes
Cas O2 Cas 31_454 32_445 113(2) yes
Cas O2 Cas 31_454 21_544 113(2) yes
Cas O2 Cas 32_445 31_454 113(2) yes
Cas O2 Cas 32_445 21_544 113(2) yes
Cas O2 Cas 21_544 31_454 113(2) yes
Cas O2 Cas 21_544 32_445 113(2) yes
Ca O3 Ca . 36_545 180 yes
Ca O3 Cas . . 0 yes
Ca O3 Cas . 36_545 180 yes
Ca O3 Ca 36_545 . 180 yes
Ca O3 Cas 36_545 . 180 yes
Ca O3 Cas 36_545 36_545 0 yes
Cas O3 Cas . 36_545 180 yes
Cas O3 Cas 36_545 . 180 yes
Ca Cas O1 . 6_554 72.3(19) yes
Ca Cas O1 . 8_545 72.3(19) yes
Ca Cas O2 . 2_545 82(2) yes
Ca Cas O2 . 11_555 82(2) yes
Ca Cas O3 . . 180 yes
O1 Cas O1 6_554 8_545 145(4) yes
O1 Cas O2 6_554 2_545 95.2(10) yes
O1 Cas O2 6_554 11_555 80.1(8) yes
O1 Cas O3 6_554 . 107.7(19) yes
O1 Cas O1 8_545 6_554 145(4) yes
O1 Cas O2 8_545 2_545 80.1(8) yes
O1 Cas O2 8_545 11_555 95.2(10) yes
O1 Cas O3 8_545 . 107.7(19) yes
O2 Cas O2 2_545 11_555 165(4) yes
O2 Cas O3 2_545 . 98(2) yes
O2 Cas O2 11_555 2_545 165(4) yes
O2 Cas O3 11_555 . 98(2) yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Ca O1 6_554 2.3900(19) yes
Ca O1 8_545 2.3900(19) yes
Ca O1 36_545 2.611(6) yes
Ca O1 38_555 2.611(6) yes
Ca O2 2_545 2.421(2) yes
Ca O2 11_555 2.421(2) yes
Ca O3 . 2.766(7) yes
Ca Cas . 0.81(9) yes
Al1 O1 6_554 1.774(4) yes
Al1 O1 36_545 1.774(4) yes
Al1 O1 43_455 1.774(4) yes
Al1 O2 . 1.718(4) yes
Al2 O1 . 1.742(2) yes
Al2 O1 3_555 1.742(2) yes
Al2 O1 36_645 1.742(2) yes
Al2 O1 38_655 1.742(2) yes
O1 O1 3_555 2.776(3) yes
O1 O1 36_645 2.877(3) yes
O1 O1 38_655 2.877(3) yes
O1 O1 15_645 2.761(3) yes
O1 O1 48_556 2.761(3) yes
O1 O2 30_555 2.963(3) yes
O1 Cas 26_555 2.51(3) yes
O2 Cas 31_454 2.393(12) yes
O2 Cas 32_445 2.393(12) yes
O2 Cas 21_544 2.393(12) yes
O3 Cas . 1.96(9) yes
O3 Cas 36_545 1.96(9) yes
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0009967
